Strength Reliability of Micro Polycrystalline Silicon ... Strength Reliability of Micro...
Embed Size (px)
Transcript of Strength Reliability of Micro Polycrystalline Silicon ... Strength Reliability of Micro...
Strength Reliability of Micro Polycrystalline Silicon Structure
Shigeru Hamada, Kenji Hasizume, Hiroyuki Nakaura and Yoshihide Sugimoto
Department of Mechanical Engineering, Faculty of Engineering, Kyushu University Japan
Polycrystalline silicon (poly-Si) structure is widely employed in the Micro-Electro- Mechanical Systems (MEMS) [Najafi, 2000; Senturia ,2000]. MEMS devices, which contain mechanical movement, have to maintain their reliability in face of external shock, thermal stress and residual stress from manufacturing processes, and fracture will begin mainly in stress concentration area. Therefore, it is necessary to build up reliability design criterion of the poly-Si structure that has stress concentration [Chen et al., 2002; Greek et al.,1997; Kapels et al., 2000; Muhlstein et al., 2004; Namazu et al., 2000; Sharpe et al., 2001; Tsuchiya et al., 1998]. However, since the size effect is large, the microscopic poly-Si depends for the strength on the effective area caused by the stress concentration of structure. Moreover, as the point peculiar to the microscopic poly-Si at the time of thinking of strength, in order that the techniques of processing the upper surface and the sidewall surface differ, it is mentioned that the surface roughness used as the source of a stress concentration differs. It depends for the strength of the microscopic poly-Si also on surface roughness. Therefore, it is necessary to deal with simultaneously the stress concentration of structure and the stress concentration by surface roughness in the case of strength evaluation. In order to clarify the bending strength and its effective area dependability of poly-Si, bending tests using micro scale cantilever beams with or without notch of several sizes are performed. Moreover, surface roughness measurement using AFM is carried out, it determines for the stress concentration by surface roughness, and a quantitative effective area is defined. Fracture origins are specified by fracture surface observation, and the validity of the effective area are shown. Finally, the static strength design criteria in consideration of scattering in strength which used two parameters, the maximum stress and an effective area, are proposed.
2. Test method
2.1 Specimen The specimens are illustrated in Fig. 1. Shapes and dimensions of the specimens are shown in Table 1. For bending tests, two types of specimens; Type-A and B are prepared. In the Type-A specimen, the notch of several sizes (1~5 [μm]) is introduced in the root section of micro- cantilever beam. In the Type-B, by the microscopic observation, the 1 [μm] corner radius is
recognized indeed in the root section of micro cantilever beam. Thickness of the specimen (h) is 3.5, 6.4 and 8.3 [μm]. The gap between the cantilever and the substrate is 2 [μm]. The poly-Si is Chemical Vapour Deposited (CVD) on single crystal silicon wafer surface, and the specimens are made from surface micromachining process. The Deep Reactive Ion Etching (DRIE) process were used for processing of the sidewall surface of 6.4, 8.3 [μm] thickness specimens. Therefore, especially in the specimen side surface made by DRIE, microscopic irregularity called “scarop” which is not seen on the upper surface. Figure 2 shows the example of the scarop for the 6.4 [μm] thickness specimen.
(a) Notched specimen (Type-A) (b) Specimen without notch (Type-B).
Fig. 1. Schematic diagram of the specimens (unit: μm), h = 3.5, 6.4, 8.3 [μm]
Specimen Type L1, μm L2, μm R, μm Type-A L15R1 20 15 1
L15R2 20 15 2 L15R3 20 15 3 L15R4 20 15 4 L15R5 20 15 5
Type-B L10 15 10 − L15 25 15 −
Table 1. Shapes and dimensions of the specimen
Fig. 2. Sidewall surface morphology of the h = 6.4 [μm] poly-Si specimen made by DRIE process
Strength Reliability of Micro Polycrystalline Silicon Structure 239
2.2 Strength test and stress analysis A dynamic ultra-micro hardness tester (Shimadzu DUH-W201) with a Berkovich diamond indenter is used for the bending tests. The test machine is for hardness tests but we can obtain the relationship between the load and the displacement with satisfactory accuracy by this machine. The test load speed is 1.421 [mN/sec.]. The bending tests are carried out at room temperature under the atmospheric environment. In order to quantify the fracture of specimens by the applied stresses in the tests, three- dimensional finite element elastic analyses are performed with Young's modulus: 148[GPa], Poisson's ratio: 0.2. The software used for this analysis is ANSYS 10.0. Figure 3 indicates the examples of FEM models of the specimens (Type-A, L15R1). For the Type-B specimen, the 1μm corner radius is taken into the model based on the microscopic observations mentioned above. The stress concentration factor of Type-B is close to that of Type-A, L15R3. The element sizes of the models are about 1μm in the overall region and are about 0.1μm in the stress concentration area near the notch root.
(a) Whole of the FEM model (1/2 model) (b) Detail of the stress concentration (notch) section of the specimen
Fig. 3. Examples of the FEM model (h = 6.4 [μm], L15R1).
2.3 Surface roughness In order to investigate the stress concentration by the shape of the microscopic surface of a specimen, surface shapes were measured using the atomic force microscope (AFM) (VEECO D-3000). The region to measure was made into 1 [μm] four quarters. The upper surfaces of the specimens were measured by scanning in the specimen longitudinal direction, and the sidewall surface of the specimens scanned and measured the scarop bottom in the specimen longitudinal direction. The maximum stress concentration factor Kt max which exists in a specimen was determined using the roughness of the measured surface. It is shown in 5.1 for details. In order to estimate the maximum stress concentration factor which exists in a specimen, the data of stress concentration factor determined by measurement was arranged using statistics of extreme [Gumbel, 1962].
2.4 Effective area The following equations thought to be able to define an effective area S. The maximum stress σmax of the structure calculated in FEM analysis and the Kt max calculated by roughness measurement are used. When the stress concentration shown in the Eq. (1) was taken into consideration, area on which the stress exceeding σmax was made into the effective area. 購鱈叩淡 判 計痛 鱈叩淡購 (1)
The S thought to expresses the effective area at the time of evaluating strength here. Within the range of an effective area, it can become fracture origin except the maximum stress working point by the stress concentration of structure by the surface roughness stress concentration.
3. Bending test results
Figure 3 shows examples of the relationship between load and displacement of the bending tests. In this figure, it is known that the polycrystalline silicon deformed elastically until final catastrophic failure in room temperature, showing a brittle nature. The relationship between load and displacement shows a little nonlinear behaviour. This is because of indentation to poly-Si of the indenter. Figure 5 shows an expression of the test results by use of maximum peak stress σmax in the notch root obtained by FEM analysis. In this figure, the plots of solid mark means the data of fracture specimens and the open mark means the data of non-fracture specimens due to the contact of free edge to the substrate surface before break. The displacement which contact occur changes with specimen, this may be because the residual stress and shape of the specimens has little difference respectively. In Fig. 5, a tendency can be seen that the plots by the σmax move down with the increase in notch radius because of the effect of the difference on the stress distribution pattern. In order to investigate the scattering in the fracture strength obtained by a bending strength test and FEM analysis, fracture strength was plotted to Weibull probability paper [Weibull, 1951]. Weibull distribution is used for strength evaluation of a brittle material like the ceramics, and it is thought that Weibull distribution can estimate the strength of the poly-Si which is brittle material. The function of two population parameters Weibull distribution can be expressed with the following equation. 繋 = な − exp 犯−畦帳 磐購台購待卑陳般 (2)
In Eq. (2), F: cumulative probability of failure, σ0: scale parameter, m: shape parameter, respectively, AE is the effective area. For Weibull plots, Eq. (2) is changed as follows. ln ln なな − 繋 = 兼岫ln 購台 − ln 購待岻 + ln 畦帳 (3)
Figure 6 shows the Weibull plots of bending strength for poly-Si. The non-fracture data are treated statistically [Johnson, 1964]. Figure 6 show the validity of using Weibull analysis for this study. Figure 7 shows the scale parameters (σ0) of this study. If shapes of the specimen are different, then effective surface area is different. Then, the scale parameter is thought to be different. Figure 7(a) shows the validity of the effective surface. Figure 7(b) shows the same result. In Fig.7, h = 3.5 [μm] specimen shows different trend. We’ll discuss about it later. Figure 8 s